{'fraction_non_alphanumeric': 0.032234297292319025, 'fraction_numerical': 0.007552035365629029, 'mean_word_length': 5.646266829865361, 'pattern_counts': {'":': 0, '<': 0, '<?xml version=': 0, '>': 0, 'https://': 0, 'lorem ipsum': 0, 'www.': 0, 'xml': 0}, 'pii_count': 0, 'substrings_counts': 0, 'word_list_counts': {'cursed_substrings.json': 0, 'profanity_word_list.json': 0, 'sexual_word_list.json': 0, 'zh_pornsignals.json': 0}}
GIWAXS: A powerful tool for perovskite photovoltaics

The power conversion efficiency (PCE) for perovskite solar cells (PSCs) now reaches 25.2%[1]. However, the perovskite materials have complex compositions and variable phases, calling for suitable characterization techniques to investigate the underlying operation and degradation mechanism. Grazing-incidence wide-angle X-ray scattering (GIWAXS) plays an important role in studying perovskite materials. GIWAXS data are generally two-dimensional diffractograms containing diffraction rings of different crystal planes. Grazing-incidence small-angle X-ray scattering (GISAXS) is similar to GIWAXS, while it has a longer detection distance than that of GIWAXS (Fig. 1(a))[2]. GISAXS enlarges the observable spatial range up to 10–100 nm and reduces the measurement sensitivity of crystallization, and it is mainly used to determine the morphology of bulk-heterojunction films in nanoscale[3, 4]. Compared to GISAXS, GIWAXS is more popular in perovskite study. This technique has several advantages as follows: (1) high signalto-noise ratio (SNR) and sensitive structural resolution; (2) nocontact and nondestructive probing; (3) abundant structural information; (4) depth resolution; (5) in-situ observation. Here, we discuss two applications of GIWAXS, i.e., the crystallographic information at steady state, and the in-situ measurement to probe the temporal information. As an important structural parameter of perovskite films, crystallographic orientation affects the optoelectronic properties and materials stability. The 2D GIWAXS diffractogram presents the Debye-Scherrer ring for certain crystallographic plane, enabling characterization of structural orientation of perovskite films. The orientation degree for crystal planes can be obtained quantitatively according to the diffraction rings along the azimuth by using Herman’s orientation function. Quasi-2D perovskites receive attention due to their variable structures, tunable composition, and relatively high stability. The insulating organic long-chain cations in quasi-2D perovskites can block carrier transport. Suitable crystal orientation can enhance the carrier transport in 2D perovskites, thus improving device performance. GIWAXS measurements give information about crystal orientation, it can also tell the stacking manner of grains at different depths, which is essential for understanding the crystallization mechanism. For example, by using GIWAXS, Choi et al. found that the nucleation and crystallization of BA2MA3Pb4I13 perovskite occurs at the gas-liquid interface during annealing, which results in the vertical alignment of 2D perovskite crystals (Fig. 1(b))[5]. They further regulated the solvent and cation to prepare highly vertically orientated 2D perovskite films[6]. Rafael et al. found that the intermediate solvent complexes provide building blocks in the formation of 2D perovskites according to GIWAXS measurements[7]. High-quality 3D perovskites tend to make strong orientation at certain azimuth angle. GIWAXS results can be used to evaluate the crystallization quality of 3D perovskite thin films. The results can also be used to guide the process optimization, as well as to clarify the relationship between crystallographic orientation and device performance. Zheng et al. regulated the preferential orientation of perovskite crystals and improved the interfacial carriers transport in the corresponding devices by substituting A-site alkali metal cations[8]. Recently, residual strain was observed in perovskite films due to the mismatch of the expansion coefficients for the substrate and perovskites, which influences the operational stability and efficiency of perovskite solar cells. Microscopically, the residual stress within the film results from a biaxial stretching of the perovskite lattice in in-plane direction. The shift of corresponding diffraction peaks at different azimuthal angles reveals the lattice tilting and stretching. By depth-resolved GIWAXS, Zhu et al. observed a gradient strain in FA-MA perovskite films (Fig. 1(c)). The performance of PSCs was improved by reducing lattice mismatch of the crystals[9]. Wang et al. replaced A-site cations on the perovskite surface by using OAI post-treatment, forming a “bone-joint” configuration, reducing surface residual stresses and thus improving humidity and thermal stability of PSCs[10]. In-situ measurement is attractive in perovskite research. It provides a rapid approach to track microstructural changes in perovskite materials, including the crystallization and aging processes. It is the key to unravel the kinetics process of perovskite materials. The formation process of perovskite crystals is not fully understood yet. The film formation process includes liquid-film gelation stage and crystallization stage. Many studies have shown that the orientation and phase structure of perovskite are already established during gelation stage. The quality of the perovskite precursor film (gel) significantly affects the final perovskite film. In-situ GIWAXS provides information for the composition evolution during spin-coating process. It also provides guidelines for preparation conditions, such as spin speed and time, dripping time of anti-solvent, etc. Amassian et al. have conducted a series of in-situ GIWAXS studies on perovskite. They observed the transition of perovskite precursors from liquid